Get Colloidal Gold essential facts below. View Videos or join the Colloidal Gold discussion. Add Colloidal Gold to your PopFlock.com topic list for future reference or share this resource on social media.
The properties of colloidal gold nanoparticles, and thus their potential applications, depend strongly upon their size and shape. For example, rodlike particles have both transverse and longitudinal absorption peak, and anisotropy of the shape affects their self-assembly.
This cranberry glass bowl was made by adding a gold salt (probably gold chloride) to molten glass.
Used since ancient times as a method of staining glass colloidal gold was used in the 4th-century Lycurgus Cup, which changes color depending on the location of light source.
During the Middle Ages, soluble gold, a solution containing gold salt, had a reputation for its curative property for various diseases. In 1618, Francis Anthony, a philosopher and member of the medical profession, published a book called Panacea Aurea, sive tractatus duo de ipsius Auro Potabili (Latin: gold potion, or two treatments of potable gold). The book introduces information on the formation of colloidal gold and its medical uses. About half a century later, English botanist Nicholas Culpepper published book in 1656, Treatise of Aurum Potabile, solely discussing the medical uses of colloidal gold.
In 1676, Johann Kunckel, a German chemist, published a book on the manufacture of stained glass. In his book Valuable Observations or Remarks About the Fixed and Volatile Salts-Auro and Argento Potabile, Spiritu Mundi and the Like, Kunckel assumed that the pink color of Aurum Potabile came from small particles of metallic gold, not visible to human eyes. In 1842, John Herschel invented a photographic process called chrysotype (from the Greek meaning "gold") that used colloidal gold to record images on paper.
Modern scientific evaluation of colloidal gold did not begin until Michael Faraday's work in the 1850s. In 1856, in a basement laboratory of Royal Institution, Faraday accidentally created a ruby red solution while mounting pieces of gold leaf onto microscope slides. Since he was already interested in the properties of light and matter, Faraday further investigated the optical properties of the colloidal gold. He prepared the first pure sample of colloidal gold, which he called 'activated gold', in 1857. He used phosphorus to reduce a solution of gold chloride. The colloidal gold Faraday made 150 years ago is still optically active. For a long time, the composition of the 'ruby' gold was unclear. Several chemists suspected it to be a gold tin compound, due to its preparation. Faraday recognized that the color was actually due to the miniature size of the gold particles. He noted the light scattering properties of suspended gold microparticles, which is now called Faraday-Tyndall effect.
With advances in various analytical technologies in the 20th century, studies on gold nanoparticles has accelerated. Advanced microscopy methods, such as atomic force microscopy and electron microscopy, have contributed the most to nanoparticle research. Due to their comparably easy synthesis and high stability, various gold particles have been studied for their practical uses. Different types of gold nanoparticle are already used in many industries, such as electronics.
The variation of scattering cross section of 100 nm-radius gold nanoparticle vs. the wavelength
Colloidal gold has been used by artists for centuries because of the nanoparticle's interactions with visible light. Gold nanoparticles absorb and scatter light resulting in colours ranging from vibrant reds to blues to black and finally to clear and colorless, depending on particle size, shape, local refractive index, and aggregation state. These colors occur because of a phenomenon called localized surface plasmon resonance (LSPR), in which conduction electrons on the surface of the nanoparticle oscillate in resonance with incident light.
Effect of size
As a general rule, the wavelength of light absorbed increases as a function of increasing nano particle size. For example, pseudo-spherical gold nanoparticles with diameters ~ 30 nm have a peak LSPR absorption at ~530 nm.[clarification needed]
Effect of local refractive index
Changes in the apparent color of a gold nanoparticle solution can also be caused by the environment in which the colloidal gold is suspended The optical properties of gold nanoparticles depends on the refractive index near the nanoparticle surface, therefore both the molecules directly attached to the nanoparticle surface (i.e. nanoparticle ligands) and/or the nanoparticle solvent both may influence observed optical features. As the refractive index near the gold surface increases, the NP LSPR will shift to longer wavelengths In addition to solvent environment, the extinction peak can be tuned by coating the nanoparticles with non-conducting shells such as silica, bio molecules, or aluminium oxide.
Effect of aggregation
When gold nano particles aggregate, the optical properties of the particle change, because the effective particle size, shape, and dielectric environment all change.
In addition to biological probes, gold nanoparticles can be transferred to various mineral substrates, such as mica, single crystal silicon, and atomically flat gold(III), to be observed under atomic force microscopy (AFM).
Drug delivery system
Gold nanoparticles can be used to optimize the biodistribution of drugs to diseased organs, tissues or cells, in order to improve and target drug delivery.
Nanoparticle-mediated drug delivery is feasible only if the drug distribution is otherwise inadequate. These cases include drug targeting of unstable (proteins, siRNA, DNA), delivery to the difficult sites (brain, retina, tumors, intracellular organelles) and drugs with serious side effects (e.g. anti-cancer agents). The performance of the nanoparticles depends on the size and surface functionalities in the particles. Also, the drug release and particle disintegration can vary depending on the system (e.g. biodegradable polymers sensitive to pH). An optimal nanodrug delivery system ensures that the active drug is available at the site of action for the correct time and duration, and their concentration should be above the minimal effective concentration (MEC) and below the minimal toxic concentration (MTC).
In cancer research, colloidal gold can be used to target tumors and provide detection using SERS (surface enhanced Raman spectroscopy) in vivo. These gold nanoparticles are surrounded with Raman reporters, which provide light emission that is over 200 times brighter than quantum dots. It was found that the Raman reporters were stabilized when the nanoparticles were encapsulated with a thiol-modified polyethylene glycol coat. This allows for compatibility and circulation in vivo. To specifically target tumor cells, the polyethylenegylated gold particles are conjugated with an antibody (or an antibody fragment such as scFv), against, e.g. epidermal growth factor receptor, which is sometimes overexpressed in cells of certain cancer types. Using SERS, these pegylated gold nanoparticles can then detect the location of the tumor.
Gold nanoparticles accumulate in tumors, due to the leakiness of tumor vasculature, and can be used as contrast agents for enhanced imaging in a time-resolved optical tomography system using short-pulse lasers for skin cancer detection in mouse model. It is found that intravenously administrated spherical gold nanoparticles broadened the temporal profile of reflected optical signals and enhanced the contrast between surrounding normal tissue and tumors.
Tumor targeting via multifunctional nanocarriers. Cancer cells reduce adhesion to neighboring cells and migrate into the vasculature-rich stroma. Once at the vasculature, cells can freely enter the bloodstream. Once the tumor is directly connected to the main blood circulation system, multifunctional nanocarriers can interact directly with cancer cells and effectively target tumors.
Gold nanoparticles have shown potential as intracellular delivery vehicles for siRNA oligonucleotides with maximal therapeutic impact.
Multifunctional siRNA-gold nanoparticles with several biomolecules: PEG, cell penetration and cell adhesion peptides and siRNA. Two different approaches were employed to conjugate the siRNA to the gold nanoparticle: (1) Covalent approach: use of thiolated siRNA for gold-thiol binding to the nanoparticle; (2) Ionic approach: interaction of the negatively charged siRNA to the modified surface of the AuNP through ionic interactions.
Gold nanoparticles show potential as intracellular delivery vehicles for antisense oligonucleotides (single and double stranded DNA) by providing protection against intracellular nucleases and ease of functionalization for selective targeting.
Gold nanorods are being investigated as photothermal agents for in-vivo applications. Gold nanorods are rod-shaped gold nanoparticles whose aspect ratios tune the surface plasmon resonance (SPR) band from the visible to near-infrared wavelength. The total extinction of light at the SPR is made up of both absorption and scattering. For the smaller axial diameter nanorods (~10 nm), absorption dominates, whereas for the larger axial diameter nanorods (>35 nm) scattering can dominate. As a consequence, for in-vivo studies, small diameter gold nanorods are being used as photothermal converters of near-infrared light due to their high absorption cross-sections. Since near-infrared light transmits readily through human skin and tissue, these nanorods can be used as ablation components for cancer, and other targets. When coated with polymers, gold nanorods have been observed to circulate in-vivo with half-lives longer than 6 hours, bodily residence times around 72 hours, and little to no uptake in any internal organs except the liver.
Despite the unquestionable success of gold nanorods as photothermal agents in preclinical research, they have yet to obtain the approval for clinical use because the size is above the renal excretion threshold. In 2019, the first NIR-absorbing plasmonic ultrasmall-in-nano architecture has been reported, and jointly combine: (i) a suitable photothermal conversion for hyperthermia treatments, (ii) the possibility of multiple photothermal treatments and (iii) renal excretion of the building blocks after the therapeutic action.
Radiotherapy dose enhancer
Considerable interest has been shown in the use of gold and other heavy-atom-containing nanoparticles to enhance the dose delivered to tumors. Since the gold nanoparticles are taken up by the tumors more than the nearby healthy tissue, the dose is selectively enhanced. The biological effectiveness of this type of therapy seems to be due to the local deposition of the radiation dose near the nanoparticles. This mechanism is the same as occurs in heavy ion therapy.
Detection of toxic gas
Researchers have developed simple inexpensive methods for on-site detection of hydrogen sulfide present in air based on the antiaggregation of gold nanoparticles (AuNPs). Dissolving into a weak alkaline buffer solution leads to the formation of HS-, which can stabilize AuNPs and ensure they maintain their red color allowing for visual detection of toxic levels of .
Gold nanoparticle based biosensor
Gold nanoparticles are incorporated into biosensors to enhance its stability, sensitivity, and selectivity. Nanoparticle properties such as small size, high surface-to-volume ratio, and high surface energy allow immobilization of large range of biomolecules. Gold nanoparticle, in particular, could also act as "electron wire" to transport electrons and its amplification effect on electromagnetic light allows it to function as signal amplifiers. Main types of gold nanoparticle based biosensors are optical and electrochemical biosensor.
Gold nanoparticles improve the sensitivity of optical sensor by response to the change in local refractive index. The angle of the incidence light for surface plasmon resonance, an interaction between light wave and conducting electrons in metal, changes when other substances are bounded to the metal surface. Because gold is very sensitive to its surroundings' dielectric constant, binding of an analyte would significantly shift gold nanoparticle's SPR and therefore allow more sensitive detection. Gold nanoparticle could also amplify the SPR signal. When the plasmon wave pass through the gold nanoparticle, the charge density in the wave and the electron I the gold interacted and resulted in higher energy response, so called electron coupling. Since the analyte and bio-receptor now bind to the gold, it increases the apparent mass of the analyte and therefore amplified the signal.
These properties had been used to build DNA sensor with 1000-fold sensitive than without the Au NP. Humidity senor was also built by altering the atom interspacing between molecules with humidity change, the interspacing change would also result in a change of the Au NP's LSPR.
Electrochemical sensor convert biological information into electrical signals that could be detected. The conductivity and biocompatibility of Au NP allow it to act as "electron wire". It transfers electron between the electrode and the active site of the enzyme. It could be accomplished in two ways: attach the Au NP to either the enzyme or the electrode. GNP-glucose oxidase monolayer electrode was constructed use these two methods. The Au NP allowed more freedom in the enzyme's orientation and therefore more sensitive and stable detection. Au NP also acts as immobilization platform for the enzyme. Most biomolecules denatures or lose its activity when interacted with the electrode. The biocompatibility and high surface energy of Au allow it to bind to a large amount of protein without altering its activity and results in a more sensitive sensor. Moreover, Au NP also catalyzes biological reactions. Gold nanoparticle under 2 nm has shown catalytic activity to the oxidation of styrene.
Gold nanoparticles have been coated with peptides and glycans for use in immunological detection methods. The possibility to use glyconanoparticles in ELISA was unexpected, but the method seems to have a high sensitivity and thus offers potential for development of specific assays for diagnostic identification of antibodies in patient sera 
Gold nanoparticles capped with organic ligands, such as alkanethiol molecules, can self-assemble into large monolayers (>cm). The particles are first prepared in organic solvent, such as chloroform or toluene, and are then spread into monolayers either on a liquid surface or on a solid substrate. Such interfacial thin films of nanoparticles have close relationship with Langmuir-Blodgett monolayers made from surfactants.
The mechanical properties of nanoparticle monolayers have been studied extensively. For 5 nm spheres capped with dodecanethiol, the Young's modulus of the monolayer is on the order of GPa. The mechanics of the membranes are guided by strong interactions between ligand shells on adjacent particles. Upon fracture, the films crack perpendicular to the direction of strain at a fracture stress of 11 2.6 MPa, comparable to that of cross-linked polymer films. Free-standing nanoparticle membranes exhibit bending rigidity on the order of 10 eV, higher than what is predicted in theory for continuum plates of the same thickness, due to nonlocal microstructural constraints such as nonlocal coupling of particle rotational degrees of freedom. On the other hand, resistance to bending is found to be greatly reduced in nanoparticle monolayers that are supported at the air/water interface, possibly due to screening of ligand interactions in a wet environment.
In many different types of colloidal gold syntheses, the interface of the nanoparticles can display widely different character - ranging from an interface similar to a self-assembled monolayer to a disordered boundary with no repeating patterns. Beyond the Au-Ligand interface, conjugation of the interfacial ligands with various functional moieties (from small organic molecules to polymers to DNA to RNA) afford colloidal gold much of its vast functionality.
After initial nanoparticle synthesis, colloidal gold ligands are often exchanged with new ligands designed for specific applications. For example, Au NPs produced via the Turkevich-style (or Citrate Reduction) method are readily reacted via ligand exchange reactions, due to the relatively weak binding between the carboxyl groups and the surfaces of the NPs. This ligand exchange can produce conjugation with a number of biomolecules from DNA to RNA to proteins to polymers (such as PEG) to increase biocompatibility and functionality. For example, ligands have been shown to enhance catalytic activity by mediating interactions between adsorbates and the active gold surfaces for specific oxygenation reactions. Ligand exchange can also be used to promote phase transfer of the colloidal particles. Ligand exchange is also possible with alkane thiol-arrested NPs produced from the Brust-type synthesis method, although higher temperatures are needed to promote the rate of the ligand detachment. An alternative method for further functionalization is achieved through the conjugation of the ligands with other molecules, though this method can cause the colloidal stability of the Au NPs to breakdown.
In many cases, as in various high-temperature catalytic applications of Au, the removal of the capping ligands produces more desirable physicochemical properties. The removal of ligands from colloidal gold while maintaining a relatively constant number of Au atoms per Au NP can be difficult due to the tendency for these bare clusters to aggregate. The removal of ligands is partially achievable by simply washing away all excess capping ligands, though this method is ineffective in removing all capping ligand. More often ligand removal achieved under high temperature or light ablation followed by washing. Alternatively, the ligands can be electrochemically etched off.
Surface structure and chemical environment
The precise structure of the ligands on the surface of colloidal gold NPs impact the properties of the colloidal gold particles. Binding conformations and surface packing of the capping ligands at the surface of the colloidal gold NPs tend to differ greatly from bulk surface model adsorption, largely due to the high curvature observed at the nanoparticle surfaces. Thiolate-gold interfaces at the nanoscale have been well-studied and the thiolate ligands are observed to pull Au atoms off of the surface of the particles to for "staple" motifs that have significant Thiyl-Au(0) character. The citrate-gold surface, on the other hand, is relatively less-studied due to the vast number of binding conformations of the citrate to the curved gold surfaces. A study performed in 2014 identified that the most-preferred binding of the citrate involves two carboxylic acids and the hydroxyl group of the citrate binds three surface metal atoms.
Health and safety
As gold nanoparticles (AuNPs) are further investigated for targeted drug delivery in humans, their toxicity needs to be considered. For the most part, it is suggested that AuNPs are biocompatible, but the concentrations at which they become toxic needs to be determined, and if those concentrations fall within the range of used concentrations. Toxicity can be tested in vitro and in vivo. In vitro toxicity results can vary depending on the type of the cellular growth media with different protein compositions, the method used to determine cellular toxicity (cell health, cell stress, how many cells are taken into a cell), and the capping ligands in solution.In vivo assessments can determine the general health of an organism (abnormal behavior, weight loss, average life span) as well as tissue specific toxicology (kidney, liver, blood) and inflammation and oxidative responses.In vitro experiments are more popular than in vivo experiments because in vitro experiments are more simplistic to perform than in vivo experiments.
Toxicity and hazards in synthesis
While AuNPs themselves appear to have low or negligible toxicity, and the literature shows that the toxicity has much more to do with the ligands rather than the particles themselves, the synthesis of them involves chemicals that are hazardous. Sodium borohydride, a harsh reagent, is used to reduce the gold ions to gold metal. The gold ions usually come from chloroauric acid, a potent acid. Because of the high toxicity and hazard of reagents used to synthesize AuNPs, the need for more "green" methods of synthesis arose.
Toxicity due to capping ligands
Some of the capping ligands associated with AuNPs can be toxic while others are nontoxic. In gold nanorods (AuNRs), it has been shown that a strong cytotoxicity was associated with CTAB-stabilized AuNRs at low concentration, but it is thought that free CTAB was the culprit in toxicity . Modifications that overcoat these AuNRs reduces this toxicity in human colon cancer cells (HT-29) by preventing CTAB molecules from desorbing from the AuNRs back into the solution.
Ligand toxicity can also be seen in AuNPs. Compared to the 90% toxicity of HAuCl4 at the same concentration, AuNPs with carboxylate termini were shown to be non-toxic. Large AuNPs conjugated with biotin, cysteine, citrate, and glucose were not toxic in human leukemia cells (K562) for concentrations up to 0.25 M. Also, citrate-capped gold nanospheres (AuNSs) have been proven to be compatible with human blood and did not cause platelet aggregation or an immune response. However, citrate-capped gold nanoparticles sizes 8-37 nm were found to be lethally toxic for mice, causing shorter lifespans, severe sickness, loss of appetite and weight, hair discoloration, and damage to the liver, spleen, and lungs; gold nanoparticles accumulated in the spleen and liver after traveling a section of the immune system.
There are mixed-views for polyethylene glycol (PEG)-modified AuNPs. These AuNPs were found to be toxic in mouse liver by injection, causing cell death and minor inflammation. However, AuNPs conjugated with PEG copolymers showed negligible toxicity towards human colon cells (Caco-2).
AuNP toxicity also depends on the overall charge of the ligands. In certain doses, AuNSs that have positively-charged ligands are toxic in monkey kidney cells (Cos-1), human red blood cells, and E. coli because of the AuNSs interaction with the negatively-charged cell membrane; AuNSs with negatively-charged ligands have been found to be nontoxic in these species.
In addition to the previously mentioned in vivo and in vitro experiments, other similar experiments have been performed. Alkylthiolate-AuNPs with trimethlyammonium ligand termini mediate the translocation of DNA across mammalian cell membranes in vitro at a high level, which is detrimental to these cells. Corneal haze in rabbits have been healed in vivo by using polyethylemnimine-capped gold nanoparticles that were transfected with a gene that promotes wound healing and inhibits corneal fibrosis.
Toxicity due to size of nanoparticles
Toxicity in certain systems can also be dependent on the size of the nanoparticle. AuNSs size 1.4 nm were found to be toxic in human skin cancer cells (SK-Mel-28), human cervical cancer cells (HeLa), mouse fibroblast cells (L929), and mouse macrophages (J774A.1), while 0.8, 1.2, and 1.8 nm sized AuNSs were less toxic by a six-fold amount and 15 nm AuNSs were nontoxic. There is some evidence for AuNP buildup after injection in in vivo studies, but this is very size dependent. 1.8 nm AuNPs were found to be almost totally trapped in the lungs of rats. Different sized AuNPs were found to buildup in the blood, brain, stomach, pancreas, kidneys, liver, and spleen.
Biosafety and biokinetics investigations on biodegradable ultrasmall-in-nano architectures have demonstrated that gold nanoparticles are able to avoid metal accumulation in organisms through escaping by the renal pathway.
Potential difference as a function of distance from particle surface.
Generally, gold nanoparticles are produced in a liquid ("liquid chemical methods") by reduction of chloroauric acid . To prevent the particles from aggregating, stabilizing agents are added. Citrate acts both as the reducing agent and colloidal stabilizer.
They can be functionalized with various organic ligands to create organic-inorganic hybrids with advanced functionality.
This simple method was pioneered by J. Turkevich et al. in 1951 and refined by G. Frens in the 1970s. It produces modestly monodisperse spherical gold nanoparticles of around 10-20 nm in diameter. Larger particles can be produced, but at the cost of monodispersity and shape. In this method, hot chloroauric acid is treated with sodium citrate solution, producing colloidal gold. The Turkevich reaction proceeds via formation of transient gold nanowires. These gold nanowires are responsible for the dark appearance of the reaction solution before it turns ruby-red.
A capping agent is used during nanoparticle synthesis to inhibit particle growth and aggregation. The chemical blocks or reduces reactivity at the periphery of the particle--a good capping agent has a high affinity for the new nuclei. Citrate ions or tannic acid function both as a reducing agent and a capping agent. Less sodium citrate results in larger particles.
Here, the gold nanoparticles will be around 5-6 nm. NaBH4 is the reducing agent, and TOAB is both the phase transfer catalyst and the stabilizing agent.
TOAB does not bind to the gold nanoparticles particularly strongly, so the solution will aggregate gradually over the course of approximately two weeks. To prevent this, one can add a stronger binding agent, like a thiol (in particular, alkanethiols), which will bind to gold, producing a near-permanent solution. Alkanethiol protected gold nanoparticles can be precipitated and then redissolved. Thiols are better binding agents because there is a strong affinity for the gold-sulfur bonds that form when the two substances react with each other. Tetra-dodecanthiol is a commonly used strong binding agent to synthesize smaller particles.
Some of the phase transfer agent may remain bound to the purified nanoparticles, this may affect physical properties such as solubility. In order to remove as much of this agent as possible, the nanoparticles must be further purified by soxhlet extraction.
This approach, discovered by Perrault and Chan in 2009, uses hydroquinone to reduce HAuCl4 in an aqueous solution that contains 15 nm gold nanoparticle seeds. This seed-based method of synthesis is similar to that used in photographic film development, in which silver grains within the film grow through addition of reduced silver onto their surface. Likewise, gold nanoparticles can act in conjunction with hydroquinone to catalyze reduction of ionic gold onto their surface. The presence of a stabilizer such as citrate results in controlled deposition of gold atoms onto the particles, and growth. Typically, the nanoparticle seeds are produced using the citrate method. The hydroquinone method complements that of Frens, as it extends the range of monodispersed spherical particle sizes that can be produced. Whereas the Frens method is ideal for particles of 12-20 nm, the hydroquinone method can produce particles of at least 30-300 nm.
This simple method, discovered by Martin and Eah in 2010, generates nearly monodisperse "naked" gold nanoparticles in water. Precisely controlling the reduction stoichiometry by adjusting the ratio of NaBH4-NaOH ions to HAuCl4-HCl ions within the "sweet zone," along with heating, enables reproducible diameter tuning between 3-6 nm. The aqueous particles are colloidally stable due to their high charge from the excess ions in solution. These particles can be coated with various hydrophilic functionalities, or mixed with hydrophobic ligands for applications in non-polar solvents. In non-polar solvents the nanoparticles remain highly charged, and self-assemble on liquid droplets to form 2D monolayer films of monodisperse nanoparticles.
Bacillus licheniformis can be used in synthesis of gold nanocubes with sizes between 10 and 100 nanometres. Gold nanoparticles are usually synthesized at high temperatures in organic solvents or using toxic reagents. The bacteria produce them in much milder conditions.
Navarro et al. method
For particles larger than 30 nm, control of particle size with a low polydispersity of spherical gold nanoparticles remains challenging. In order to provide maximum control on the NP structure, Navarro and co-workers used a modified Turkevitch-Frens procedure using sodium acetylacetonate as the reducing agent and sodium citrate as the stabilizer.
Another method for the experimental generation of gold particles is by sonolysis. The first method of this type was invented by Baigent and Müller. This work pioneered the use of ultrasound to provide the energy for the processes involved and allowed the creation of gold particles with a diameter of under 10 nm. In another method using ultrasound, the reaction of an aqueous solution of HAuCl4 with glucose, the reducing agents are hydroxyl radicals and sugar pyrolysisradicals (forming at the interfacial region between the collapsing cavities and the bulk water) and the morphology obtained is that of nanoribbons with width 30-50 nm and length of several micrometers. These ribbons are very flexible and can bend with angles larger than 90°. When glucose is replaced by cyclodextrin (a glucose oligomer), only spherical gold particles are obtained, suggesting that glucose is essential in directing the morphology toward a ribbon.
Block copolymer-mediated method
An economical, environmentally benign and fast synthesis methodology for gold nanoparticles using block copolymer has been developed by Sakai et al. In this synthesis methodology, block copolymer plays the dual role of a reducing agent as well as a stabilizing agent. The formation of gold nanoparticles comprises three main steps: reduction of gold salt ion by block copolymers in the solution and formation of gold clusters, adsorption of block copolymers on gold clusters and further reduction of gold salt ions on the surfaces of these gold clusters for the growth of gold particles in steps, and finally its stabilization by block copolymers. But this method usually has a limited-yield (nanoparticle concentration), which does not increase with the increase in the gold salt concentration. Ray et al. improved this synthesis method by enhancing the nanoparticle yield by manyfold at ambient temperature.
^Antonii F (1618). Panacea aurea sive Tractatus duo de ipsius auro potabili. Ex Bibliopolio Frobeniano.
^Culpeper N (1657). Mr. Culpepper's Treatise of aurum potabile Being a description of the three-fold world, viz. elementary celestial intellectual containing the knowledge necessary to the study of hermetick philosophy. Faithfully written by him in his life-time, and since his death, published by his wife. London.
^Kunckel von Löwenstern J (1678). Utiles observationes sive animadversiones de salibus fixis et volatilibus, auro et argento potabili (etc.). Austria: Wilson.
^Anderson ML, Morris CA, Stroud RM, Merzbacher CI, Rolison DR (1999-02-01). "Colloidal Gold Aerogels: Preparation, Properties, and Characterization". Langmuir. 15 (3): 674-681. doi:10.1021/la980784i.
^ abLink S, El-Sayed MA (1999-05-01). "Size and Temperature Dependence of the Plasmon Absorption of Colloidal Gold Nanoparticles". The Journal of Physical Chemistry B. 103 (21): 4212-4217. CiteSeerX10.1.1.596.6328. doi:10.1021/jp984796o.
^ abGhosh SK, Nath S, Kundu S, Esumi K, Pal T (2004-09-01). "Solvent and Ligand Effects on the Localized Surface Plasmon Resonance (LSPR) of Gold Colloids". The Journal of Physical Chemistry B. 108 (37): 13963-13971. doi:10.1021/jp047021q.
^ abUnderwood S, Mulvaney P (1994-10-01). "Effect of the Solution Refractive Index on the Color of Gold Colloids". Langmuir. 10 (10): 3427-3430. doi:10.1021/la00022a011.
^Xing S, Tan LH, Yang M, Pan M, Lv Y, Tang Q, Yang Y, Chen H (2009-05-12). "Highly controlled core/shell structures: tunable conductive polymer shells on gold nanoparticles and nanochains". Journal of Materials Chemistry. 19 (20): 3286. doi:10.1039/b900993k. S2CID96293198.
^Ghosh SK, Pal T (November 2007). "Interparticle coupling effect on the surface plasmon resonance of gold nanoparticles: from theory to applications". Chemical Reviews. 107 (11): 4797-862. doi:10.1021/cr0680282. PMID17999554. S2CID46326525.
^Electron microscopy: principles and techniques for biologists (2nd ed.). Jones and Bartlett. October 1998. ISBN978-0-7637-0192-5.
^Hunter EE (September 1993). Practical electron microscopy : a beginner's illustrated guide (2nd ed.). Cambridge University Press. ISBN978-0-521-38539-8.
^Electron microscopy: methods and protocols. Methods in Molecular Biology (2nd ed.). Humana Press. February 2007. ISBN978-1-58829-573-6.
^Romano EL, Romano M (1977). "Staphylococcal protein a bound to colloidal gold: A useful reagent to label antigen-antibody sites in electron microscopy". Immunochemistry. 14 (9-10): 711-715. doi:10.1016/0019-2791(77)90146-X.
^Grobelny J, DelRio FW, Pradeep N, Kim DI, Hackley VA, Cook RF (2011). "Size measurement of nanoparticles using atomic force microscopy". In McNeil SE (ed.). Characterization of nanoparticles intended for drug delivery. Humana Press. pp. 71-82. ISBN978-1-60327-198-1.
^Qian X, Peng XH, Ansari DO, Yin-Goen Q, Chen GZ, Shin DM, Yang L, Young AN, Wang MD, Nie S (January 2008). "In vivo tumor targeting and spectroscopic detection with surface-enhanced Raman nanoparticle tags". Nature Biotechnology. 26 (1): 83-90. doi:10.1038/nbt1377. PMID18157119. S2CID15309464.
^Sajjadi AY, Suratkar AA, Mitra KK, Grace MS (2012). "Short-Pulse Laser-Based System for Detection of Tumors: Administration of Gold Nanoparticles Enhances Contrast". J. Nanotechnol. Eng. Med. 3 (2): 021002. doi:10.1115/1.4007245.
^Giljohann DA, Seferos DS, Prigodich AE, Patel PC, Mirkin CA. Gene regulation with polyvalent siRNA-nanoparticle conjugates. J Am Chem Soc 2009;131:2072-2073.
^Niidome T, Yamagata M, Okamoto Y, Akiyama Y, Takahashi H, Kawano T, Katayama Y, Niidome Y (September 2006). "PEG-modified gold nanorods with a stealth character for in vivo applications". Journal of Controlled Release. 114 (3): 343-7. doi:10.1016/j.jconrel.2006.06.017. PMID16876898.
^Wang J, Polsky R, Xu D (2001). "Silver-Enhanced Colloidal Gold Electrochemical Stripping Detection of DNA Hybridization". Langmuir. 17 (19): 5739. doi:10.1021/la011002f.
^Wang J, Xu D, Polsky R (April 2002). "Magnetically-induced solid-state electrochemical detection of DNA hybridization". Journal of the American Chemical Society. 124 (16): 4208-9. doi:10.1021/ja0255709. PMID11960439.
^Daniel MC, Astruc D (January 2004). "Gold nanoparticles: assembly, supramolecular chemistry, quantum-size-related properties, and applications toward biology, catalysis, and nanotechnology". Chemical Reviews. 104 (1): 293-346. doi:10.1021/cr030698+. PMID14719978. S2CID29293663.
^Hu M, Chen J, Li ZY, Au L, Hartland GV, Li X, Marquez M, Xia Y (November 2006). "Gold nanostructures: engineering their plasmonic properties for biomedical applications". Chemical Society Reviews. 35 (11): 1084-94. doi:10.1039/b517615h. PMID17057837. S2CID2259806.
^Link S, El-Sayed MA (1996). "Spectral Properties and Relaxation Dynamics of Surface Plasmon Electronic Oscillations in Gold and Silver Nanodots and Nanorods". J. Phys. Chem. B. 103 (40): 8410. doi:10.1021/jp9917648. S2CID40012876.
^Mulvaney, P. (1996). "Surface Plasmon Spectroscopy of Nanosized Metal Particles". Langmuir. 12 (3): 788. doi:10.1021/la9502711.
^Lin HY, Chen CT, Chen YC (October 2006). "Detection of phosphopeptides by localized surface plasma resonance of titania-coated gold nanoparticles immobilized on glass substrates". Analytical Chemistry. 78 (19): 6873-8. doi:10.1021/ac060833t. PMID17007509. S2CID13373307.
^He L, Musick MD, Nicewarner SR, Salinas FG (2000). "Colloidal Au-Enhanced Surface Plasmon Resonance for Ultrasensitive Detection of DNA Hybridization". Journal of the American Chemical Society. 122 (38): 9071. doi:10.1021/ja001215b.
^Brown KR, Fox P, Natan MJ (1996). "Morphology-Dependent Electrochemistry of Cytochromecat Au Colloid-Modified SnO2Electrodes". Journal of the American Chemical Society. 118 (5): 1154. doi:10.1021/ja952951w.
^Gole A, Dash C, Ramakrishnan V, Sainkar SR, Mandale AB, Rao M, Sastry M (2001). "Pepsin-Gold Colloid Conjugates: Preparation, Characterization, and Enzymatic Activity". Langmuir. 17 (5): 1674. doi:10.1021/la001164w.
^Gole A, Vyas S, Phadtare S, Lachke A, Sastry M (2002). "Studies on the formation of bioconjugates of Endoglucanase with colloidal gold". Colloids and Surfaces B: Biointerfaces. 25 (2): 129. doi:10.1016/s0927-7765(01)00301-0.
^Perumal S, Hofmann A, Scholz N, Rühl E, Graf C (April 2011). "Kinetics study of the binding of multivalent ligands on size-selected gold nanoparticles". Langmuir. 27 (8): 4456-64. doi:10.1021/la105134m. PMID21413796.
^Niu Z, Li Y (2014-01-14). "Removal and Utilization of Capping Agents in Nanocatalysis". Chemistry of Materials. 26 (1): 72-83. doi:10.1021/cm4022479.
^Häkkinen H, Walter M, Grönbeck H (May 2006). "Divide and protect: capping gold nanoclusters with molecular gold-thiolate rings". The Journal of Physical Chemistry B. 110 (20): 9927-31. doi:10.1021/jp0619787. PMID16706449.
^Park JW, Shumaker-Parry JS (February 2014). "Structural study of citrate layers on gold nanoparticles: role of intermolecular interactions in stabilizing nanoparticles". Journal of the American Chemical Society. 136 (5): 1907-21. doi:10.1021/ja4097384. PMID24422457.
^Perala SR, Kumar S (August 2013). "On the mechanism of metal nanoparticle synthesis in the Brust-Schiffrin method". Langmuir. 29 (31): 9863-73. doi:10.1021/la401604q. PMID23848382.
^ abcAlkilany AM, Nagaria PK, Hexel CR, Shaw TJ, Murphy CJ, Wyatt MD (March 2009). "Cellular uptake and cytotoxicity of gold nanorods: molecular origin of cytotoxicity and surface effects". Small. 5 (6): 701-8. doi:10.1002/smll.200801546. PMID19226599.
^Takahashi H, Niidome Y, Niidome T, Kaneko K, Kawasaki H, Yamada S (January 2006). "Modification of gold nanorods using phosphatidylcholine to reduce cytotoxicity". Langmuir. 22 (1): 2-5. doi:10.1021/la0520029. PMID16378388.
^ abcGoodman CM, McCusker CD, Yilmaz T, Rotello VM (June 2004). "Toxicity of gold nanoparticles functionalized with cationic and anionic side chains". Bioconjugate Chemistry. 15 (4): 897-900. doi:10.1021/bc049951i. PMID15264879.
^Connor EE, Mwamuka J, Gole A, Murphy CJ, Wyatt MD (March 2005). "Gold nanoparticles are taken up by human cells but do not cause acute cytotoxicity". Small. 1 (3): 325-7. doi:10.1002/smll.200400093. PMID17193451.
^Cho WS, Cho M, Jeong J, Choi M, Cho HY, Han BS, Kim SH, Kim HO, Lim YT, Chung BH, Jeong J (April 2009). "Acute toxicity and pharmacokinetics of 13 nm-sized PEG-coated gold nanoparticles". Toxicology and Applied Pharmacology. 236 (1): 16-24. doi:10.1016/j.taap.2008.12.023. PMID19162059.
^Boisselier E, Astruc D (June 2009). "Gold nanoparticles in nanomedicine: preparations, imaging, diagnostics, therapies and toxicity". Chemical Society Reviews. 38 (6): 1759-82. doi:10.1039/b806051g. PMID19587967.
^Cassano, Domenico; Summa, Maria; Pocoví-Martínez, Salvador; Mapanao, Ana-Katrina; Catelani, Tiziano; Bertorelli, Rosalia; Voliani, Valerio (February 2019). "Biodegradable Ultrasmall-in-Nano Gold Architectures: Mid-Period In Vivo Distribution and Excretion Assessment". Particle & Particle Systems Characterization. 36 (2): 1800464. doi:10.1002/ppsc.201800464.
^Turkevich J, Stevenson PC, Hillier J (1951). "A study of the nucleation and growth processes in the synthesis of colloidal gold". Discuss. Faraday Soc. 11: 55-75. doi:10.1039/df9511100055. S2CID97664009.
^Kimling J, Maier M, Okenve B, Kotaidis V, Ballot H, Plech A (August 2006). "Turkevich method for gold nanoparticle synthesis revisited". The Journal of Physical Chemistry B. 110 (32): 15700-7. doi:10.1021/jp061667w. PMID16898714. S2CID11729630.
^Pong BK, Elim HI, Chong JX, Trout BL, Lee JY (2007). "New Insights on the Nanoparticle Growth Mechanism in the Citrate Reduction of Gold(III) Salt: Formation of the Au Nanowire Intermediate and Its Nonlinear Optical Properties". J. Phys. Chem. C. 111 (17): 6281-6287. doi:10.1021/jp068666o.
^Niu Z, Li Y (2014). "Removal and Utilization of Capping Agents in Nanocatalysis". Chemistry of Materials. 26: 72-83. doi:10.1021/cm4022479.
^Fang Y, Tan J, Lan T, Foo SG, Pyun DG, Lim S, Kim D (2018). "Universal one-pot, one-step synthesis of core-shell nanocomposites with self-assembled tannic acid shell and their antibacterial and catalytic activities". Journal of Applied Polymer Science. 135 (6): 45829. doi:10.1002/app.45829.
^Fang Y, Tan J, Choi H, Lim S, Kim D (2018). "Highly sensitive naked eye detection of Iron (III) and H2O2 using poly-(tannic acid) (PTA) coated Au nanocomposite". Sensors and Actuators B: Chemical. 259: 155-161. doi:10.1016/j.snb.2017.12.031.
^Brust M, Walker M, Bethell D, Schiffrin DJ, Whyman R (1994). "Synthesis of Thiol-derivatised Gold Nanoparticles in a Two-phase Liquid-Liquid System". Chem. Commun. (7): 801-802. doi:10.1039/C39940000801.
^Gao J, Huang X, Liu H, Zan F, Ren J (March 2012). "Colloidal stability of gold nanoparticles modified with thiol compounds: bioconjugation and application in cancer cell imaging". Langmuir. 28 (9): 4464-71. doi:10.1021/la204289k. PMID22276658.
^Bekalé, Laurent, Saïd Barazzouk, and Surat Hotchandani. "Beneficial Role of Gold Nanoparticles as Photoprotector of Magnesium Tetraphenylporphyrin." SpringerReference (n.d.): n. pag. Web. 14 Nov. 2016.
^Perrault SD, Chan WC (December 2009). "Synthesis and surface modification of highly monodispersed, spherical gold nanoparticles of 50-200 nm". Journal of the American Chemical Society. 131 (47): 17042-3. doi:10.1021/ja907069u. PMID19891442.
^Martin MN, Basham JI, Chando P, Eah SK (May 2010). "Charged gold nanoparticles in non-polar solvents: 10-min synthesis and 2D self-assembly". Langmuir. 26 (10): 7410-7. doi:10.1021/la100591h. PMID20392108. A 3-min demonstration video for the Martin synthesis method is available at YouTube
^Kalishwaralal K, Deepak V, Ram Kumar Pandian S, Gurunathan S (November 2009). "Biological synthesis of gold nanocubes from Bacillus licheniformis". Bioresource Technology. 100 (21): 5356-8. doi:10.1016/j.biortech.2009.05.051. PMID19574037.
^Navarro JR, Lerouge F, Cepraga C, Micouin G, Favier A, Chateau D, Charreyre MT, Lanoë PH, Monnereau C, Chaput F, Marotte S, Leverrier Y, Marvel J, Kamada K, Andraud C, Baldeck PL, Parola S (November 2013). "Nanocarriers with ultrahigh chromophore loading for fluorescence bio-imaging and photodynamic therapy". Biomaterials. 34 (33): 8344-51. doi:10.1016/j.biomaterials.2013.07.032. PMID23915950.
^Zhang J, Du J, Han B, Liu Z, Jiang T, Zhang Z (February 2006). "Sonochemical formation of single-crystalline gold nanobelts". Angewandte Chemie. 45 (7): 1116-9. doi:10.1002/ange.200503762. PMID16389606.
^Sakai T, Alexandridis P (April 2005). "Mechanism of gold metal ion reduction, nanoparticle growth and size control in aqueous amphiphilic block copolymer solutions at ambient conditions". The Journal of Physical Chemistry B. 109 (16): 7766-77. doi:10.1021/jp046221z. PMID16851902.
^Ray D, Aswal VK, Kohlbrecher J (March 2011). "Synthesis and Characterization of High Concentration Block Copolymer-Mediated Gold Nanoparticles". Langmuir. 27 (7): 4048-56. doi:10.1021/la2001706. PMID21366279.
Boisselier E, Astruc D (June 2009). "Gold nanoparticles in nanomedicine: preparations, imaging, diagnostics, therapies and toxicity". Chemical Society Reviews. 38 (6): 1759-82. doi:10.1039/b806051g. PMID19587967.